EUROPEAN ORGANIZATION FOR NUCLEAR RESEARCH
Addendum to the ISOLDE and Neutron Time-of-Flight Committee
Emission Mössbauer spectroscopy of advanced materials for opto- and
4 th January 2012
H. P. Gunnlaugsson 1 , S. Ólafsson 2 , K. Bharuth-Ram 3 , J. G. Correia 4 , H. P. Gíslason 2 , K.
Johnston 5 , G. Langouche 6 , M. B. Madsen 7 , R. Mantovan 8 , H. Masenda 9 , A. Mesli 10 , T. E.
Mølholt 2 , D. Naidoo 9 , U. Wahl 4 , G. Weyer 1
1 Department of Physics and Astronomy, Aarhus University, DK-8000 Århus C, Denmark
2 Science Institute, University of Iceland, Dunhaga 3, IS-107 Reykjavík, Iceland
3 iThemba LABS, P.O. Box 722, Somerset West 7129, South Africa
4 Departamento Física, Instituto Tecnológico e Nuclear, Sacavém, Portugal
5 EP Division, CERN, CH-1211 Geneva 23, Switzerland
6 Instituut voor Kern-en Stralings fysika, University of Leuven, B-3001 Leuven, Belgium
7 Niels Bohr Institute, Universtity of Copenhagen, DK-2100 Copenhagen Oe, Denmark
8 CNR-IMM MDM Laboratory, Via C. Olivetti 2, 20041 Agrate Brianza (MB), Italy
9 School of Physics, University of the Witwatersrand, WITS 2050, South Africa
10 IM2NP, Aix- , Marseille University, France
Spokesperson(s): H. P. Gunnlaugsson (email@example.com) S. Ólafsson (firstname.lastname@example.org)
Local contact: Karl Johnston (email@example.com)
In 2010, 15 shifts were awarded to the proposal entitled “Emission Mössbauer spectroscopy
of advanced materials for opto- and nano- electronics”, for investigations on
(1) Paramagnetic relaxations in compound semiconductors
(2) Vacancy diffusion in group IV semiconductors.
On both subjects, major progress has been made, but after two years, many questions are still
open, and we wish to propose a continuation of our investigations to derive solid conclusions
on many aspects of these investigations.
Requested shifts: 17 shifts, (split into 1-4 runs over 1 year)
1 The IS501 experiment
In 2010, 15 shifts were awarded to the proposal entitled “Emission Mössbauer spectroscopy
of advanced materials for opto- and nano- electronics”. The proposal focussed on four types
(1) Paramagnetic relaxations in compound semiconductors
(2) Vacancy diffusion in group IV semiconductors
(3) Doping of Si-nano-particles
(4) Investigation of phase change mechanisms in chalcogenides.
The INTC committee gave priority to the first two investigations, and based on the
evaluation, (3) was dropped and (4) only taken as opportunistic science of low priority in our
In this addendum, we apply for beam time in 2012 to complete studies on outstanding
questions on the two first subjects. In the following sections, the research fields are described,
a brief status report after two years of the IS501 experiment is presented, and lastly we
summarize our requirements to complete the picture(s) resulting from the investigations that
have been done.
Details from beam reports and beam usage are given in section 8.
2 Paramagnetic relaxation in compound semiconductors
Dilute magnetic semiconductors obtained by partial replacement of the cations in
conventional semiconductors by transition-metal ions have been of major interest as potential
innovative semiconductor-compatible magnetic materials for spintronic applications.
Theoretical predictions of Dietl et al. [Dietl00] of room temperature ferromagnetism (RTFM)
in ZnO (and p-type GaN) prompted a plethora of experimental studies of RTFM in ZnO and
other metal oxides. Some experiments have observed RTFM (see e.g. [Jung02]) while others
have not, and the origin of magnetism of transition-metal doped ZnO is controversial
[Koji06, Osgur05] and There are inconsistent reports in the literature. Recently, the role
played by defects in dilute magnetism have been discussed by many authors
[Kapilashrami09, Khalid09, Wang08, Wang09], while others have suggested that the
observed magnetic ordering may be due to unintentional precipitation, formation of
secondary phases or misinterpretation of data [Potzger09, Zhou09].
By employing 57 Mn (T½ = 1.5 min.) to populate the Mössbauer state of 57 Fe, we have
demonstrated that dilute Fe upon implantation occupies paramagnetic sites in ZnO and
related model systems (MgO, -Al2O3 [Gunnlaugsson10a]). Using the 57 Mn beam at
ISOLDE we are able to study the material at local Fe concentrations < 10 -4 at. % and any
concerns about putative precipitation are obviated. If magnetic order exists in the ZnO, our
results show that this has nothing to do with the dilute iron impurities. Representative
emission MS results for ZnO in an external magnetic field are shown in Fig. 1.
Fig. 1: Room temperature Mössbauer spectra of 57 Fe obtained after implantation of 57 Mn in ZnO. The
spectra are obtained in ~0.6 T external magnetic field oriented as indicated with respect to the direction
of propagation of the -quanta (adapted from [Gunnlaugsson10a]).
In the spectrum measured in external magnetic field at 60º, small features are seen at v ~ -3
mm/s and v ~ 2.5 mm/s that are clearly absent in the spectrum measured in magnetic field at
0º. This is characteristic for the disappearance of the lines belonging to the mI = 0 transition
for a SZ = ±3/2 electronic state. Such a state can only exist in paramagnets (ferromagnets have
only a spectrum resembling the spectrum from the SZ = ±5/2 electronic state). This result
shows that the electronic spin of the Fe 3+ atom is not coupled to lattice defects from the
implantation nor to the lattice, which would result in fast spin-spin or spin-lattice relaxations.
The absence of such couplings shows that the Fe 3+ atoms are unlikely to act as the seed
needed for the proposed (long range) ferromagnetism.
2.2 Current status
As a part of the IS501 experiment, paramagnetism of Fe 3+ has been verified in several
model systems by measurements performed in an external magnetic field. Already published
data includes MgO and -Al2O3 [Gunnlaugsson10b, Gunnlaugsson10c] (more data on several
additional systems awaits publications). A method to extract the temperature dependent spinlattice
relaxation rates of Fe 3+ in dilute systems has been developed [Mølholt10] which is
sensitive to relaxation rate in the range of −1 = 4×10 6 − 1×10 8 s −1 . This method has been
applied for MgO [Mølholt10], -Al2O3 [Gunnlaugsson10b] and ZnO [Mølholt12] (more data
awaits publication). In this context, ZnO has shown some peculiar and interesting properties
(cf. Fig. 2).
Relaxation rate 1/ (s -1 )
-Al 2O 3
70 100 300
Fig. 2: Spin-lattice relaxation rates of Fe 3+ obtained for the materials indicated (from [Molholt12]).
The spin-lattice relaxation rate of Fe 3+ in ZnO does not follow the T 2 dependence expected
for temperatures T > D/2, where D is the Debye temperature (see e.g. theoretical overview
in [Mørup11] and [Srivastava80] and discussed in [Mølholt12]). Moreover, ZnO has a lower
Debye temperature than MgO and -Al2O3 illustrating further this inconsistency with theory.
The reason for this is at present unknown, but the experimental data has been provided to the
scientific community [Mølholt12]. Preliminary analyses of paramagnetic relaxations of Fe 3+
TiO2, SiO2, ZrO2, SrTiO3 and GaN (unpublished results) also show the T 2 temperature
dependence. These results require further investigation before publication. It should be
emphasized that the study of these spin-lattice relaxation effects is only possible when the
local concentration of Fe is below 10 -2 at. %. At higher concentrations, spin-spin relaxations
start to play a role, and severely hamper the interpretation of the data. Therefore our studies at
ISOLDE/CERN (employing probes at concentration < 10 -4 at. %) offers a unique opportunity
to provide additional data to the scientific community on effects not explained by current
theories on spin-lattice relaxation rates that are at dilution levels and temperatures that are
outside the reach of any other experimental method.
Another peculiarity regarding ZnO is that the concentration of paramagnetic Fe 3+
complexes increases with implantation fluence [Mølholt09], which may be due to
implantation induced changes in the Fermi level, or due to pairing of Fe with structural
defects. With good datasets acquired under different fluences, we have verified that the
former explanation (implantation induced changes of the Fermi level) is indeed correct
[Mantovan12]. ZnO is intrinsically n-type, and this feature suggests that the Fermi level
moves toward the mid-gab under implantation conditions (implant isolation [Kucheyev03]).
We have furthermore demonstrated that this change in the Fermi level is unstable at room
temperature on a time scale of weeks [Naidoo12] and may contribute to explaining some
inconsistencies in the literature regarding this material.
In 2010, a beam of 57 Co (T½ = 272 d) was developed at ISOLDE. Unfortunately, it
contained high level of impurities (99% of the beam is stable 57 Fe), which hamper
significantly the usefulness of this beam. In the case of ZnO, we were able to make use of the
57 Fe contamination in the beam as it allowed us to bridge the fluence gap between our
ISOLDE data using 57 Mn (maximum dose 10 12 cm -2 ) and laboratory measurements utilizing
stable 57 Fe (~10 16 cm -2 ) [Potzger06]. Measurements on a ZnO sample implanted with 57 Co (5-
6)×10 12 cm -2 + 57 Fe (5-6)×10 14 cm -2 showed that Co/Fe enter damage sites of interstitial
character (low Debye temperature) upon implantation fluence > 10 13 cm -2
[Gunnlaugsson12a]. It was moreover shown that this Fe in interstitial damage sites was
mobilized with annealing at T = 500°C to form precipitates. Such precipitates would easily be
detected with magnetization measurements, giving an alternative explanation of the
observation of magnetism in these systems. Furthermore, these measurements resolved the
apparent inconsistency in earlier Mössbauer data.
Having understood the role of the Fe 3+ state in ZnO, the parameters of the damage
component in ZnO and how to interpret slow paramagnetic relaxation, much more data are
planned to be published soon. This includes: In-growth of the Fe 3+ state [Mantovan12],
annealing of the Fe 3+ state [Naidoo12], damage in pre-implanted samples [Gunnlaugsson12b]
and paramagnetic relaxation in other types of materials [Publication schedule to be
Our results show that if diluted magnetism exists in any of the systems investigated, it has
at least nothing to do with the 3d metal impurities. Some theoretical calculations suggest that
defects may carry a magnetic moment [Wang08]. We tested this hypothesis by applying
119m Sn Mössbauer spectroscopy following implantation of 119 In. The 119m Sn probe is by factor
of ~ 4 more sensitive to magnetic interactions than 57 Fe (see e.g. listing of the properties of
Mössbauer nuclei in [MossOrg_Periodic]). The results corroborate the results obtained with
57 Mn that there is no strong magnetic interactions from nearby defects in ZnO, MgO and -
Al2O3. However, an even stranger conclusion came from this work (cf. Fig. 3).
Relative emission (arb. units)
-6 -4 -2 0 2 4 6
Fig. 3: 119 Sn Mössbauer spectra obtained after implantation of 119 In into a ZnO single crystal held at the
temperatures indicated. The total dose is ~10 10 119 In/cm 2 per measurement.
At low temperatures, some of the Sn is observed in the expected 2+ state, but at elevated
temperatures, Sn 4+ is observed. This is in contradiction with the results obtained with 57 Mn,
where one finds that above room temperature and for fluence < 10 11 cm -2 , Fe occupies regular
lattice sites and is observed as Fe 2+ by simple replacement of Zn 2+ . Similar results were
obtained in -Al2O3 and MgO. One straightforward explanation of this finding is that the
relatively large In ion cannot simply exchange the metal ion, and hence is in a site with a
charge compensating metal vacancy as the next nearest neighbour.
This result and its interpretation is of fundamental importance for several reasons:
(1) 111 In is commonly used as a probe for perturbed angular correlation (PAC)
experiments (see e.g. [Dogra09] and references therein). It is often assumed that the
probe upon annealing occupies regular substitutional sites. Our results suggest that
this assumption is not necessarily correct, and it would be of interest to be able to
investigate this in more detail.
(2) In + N co-doping of ZnO has been suggested as a method to obtain p-type doping in
ZnO [Ye09]. If we prove that In implanted into ZnO does not lead to a simple
replacement of Zn, it might help in a further theoretical and/or experimental
endeavour to use such co-doping
Although the quality of the 119 In beam in 2011 was below usefulness, we were able to
generate one spectrum after implantation in ZnSe.
Relative emission (arb. Units)
119 In → 119 Sn
Sn 2+ Sn 0+ Sn 4+
-9 -6 -3 0 3 6 9
nn = 2.45 Å
nn = 2.1 Å
nn = 1.97 Å
Fig. 4: 119 Sn Mössbauer spectra obtained after implantation of 119 In into the materials indicated, all held
In MgO and in ZnO, one observes a broadened line due to Sn 4+ , but in ZnSe, the probe atom
enters a regular lattice site (no additional broadening). A possible, simple interpretation is
that in MgO and ZnO the In atom is present on a site with a vacancy on the metal site..
2.3 Proposed methods and experimental plan
As a follow up on the results outlined above, we propose the studies described below which
is a reasonable goal to reach within the one year before the 2013 shut-down.
(1) What is the reason for the unusual temperature dependence of the paramagnetic
relaxation rates in ZnO?
(2) The lattice location/properties of In in oxides/group II-VI´s
For (1), we plan to expand on our current list of oxides to obtain more data on slow
paramagnetic relaxations of Fe 3+ using implantation of 57 Mn. This would include temperature
scans (90-600 K) in relevant oxides (e.g. SrO, BaO), selected compound oxides (BaTiO3,…)
and selected group II-VI semiconductors (Zn, Cd)(S, Se, Te). At least 5 different compounds
would be investigated, and in selected cases angular dependent measurements in external
magnetic field included together with time dependent measurements to document any
possible metastable defects. Assuming “normal” intensity of the 57 Mn beam (usually ~2×10 8
ions/s), recording of a reasonable high temperature series takes on the average 1 hour per
sample, and 1.25 hour for a cold series. Good angular dependent measurements in external
magnetic field take ~2 hour per sample. Thus for five different compositions, roughly 2 shifts
would be required.
For (2), we propose using 119 In and 119m Sn implantations. Here it is possible to make use of
the dataset obtained in (1) because 57 Fe Mössbauer spectroscopy better determines the
annealing reactions of implantation damage due to its higher sensitivity to quadrupole
interactions. For 119 In, temperature scans (90-600 K) in some of the same types of samples
used in (1) should be performed. Assuming laser ionization and 4×10 7 119 In/µC (see below),
the total time needed for this part is (7-9 temperature steps, 20 minutes per step, in at least 5
types of materials) ~13 hours (1.6 shifts). 119m Sn has not previously been applied to study
these systems at all, so no data exists. According to the beam estimates (~1×10 9 119m Sn/s, can
be expected, see below), it will take roughly an hour to prepare the sample with 10 13 cm -2 and
an activity of 0.15 Mbq (4 µCi) which would be suitable for off-line Mössbauer
measurements and PAC measurements. 119m Sn should be implanted into at least 12 samples,
among them ZnO, MgO, SrO, BaO, -Al2O3, SiO2, ((Zn, Cd)(S, Se, Te)). In the case of some
of those (ZnO and others showing high damage resistance), higher doses should be applied
and also implantations at elevated temperatures. Good suite of 119m Sn implanted samples that
can then be used in measurements during the long shut-down is obtained within 3 shifts.
Upon completing the experimental plan (and off-line measurements) we will have obtained
more data on paramagnetic relaxations of Fe 3+ in oxides and compound semiconductors,
giving unique dataset and pointers to the peculiar behaviour of Fe 3+ in ZnO. Using this
dataset, we will have documented the lattice properties of In/Sn in oxides and group II-VI
semiconductors and answered specific questions such as whether In ions enter regular lattice
sites upon implantation, whether it is the chemical nature of In that prevents it to enter regular
lattice sites and whether it is possible to construct annealing procedures for 119m Sn implanted
samples in order to incorporate Sn into regular lattice sites.
3 Vacancy diffusion in group IV semiconductors
Silicon has maintained its position as the most important material in semiconductor
technology for decades and is probably the most studied material in the world. It is difficult
to avoid transition metal ions completely during crystal growth. They have deep levels in the
silicon bandgap and act as recombination centres. Transition metal impurities in general have
low solubility, and are fast diffusers in silicon, and have received much attention in the
literature (see e.g. review [Istratov99]). In previous experiments at ISOLDE we have
concentrated on the physics of iron impurities in Si and other group IV semiconductors using
57 Mn (Experiments IS359 and IS426) (see [MossbColl]). In the present proposal we
investigate some of the intrinsic properties of the silicon substrate making use of the
implanted 57 Mn probe
Among fundamental open issues regarding the properties of silicon is the diffusivity and
nature of the mono-vacancy at elevated temperatures. This behaviour of the mono-vacancy is
a determining factor for the diffusivity of many species in the material, and understanding its
behaviour can lead to better methods to model the material at processing temperatures. In this
context, we have the unique situation that 57 Mn (T½ = 1.5 min.) decays to the Mössbauer
state of 57 Fe giving the Fe atom recoil of average energy ER = 40 eV. This creates an
interstitial Fe atom and a mono-vacancy in its vicinity. Some of the interstitial Fe atoms
recombine with the vacancies at temperatures above 600 K, allowing us to study the
behaviour of the vacancy at temperatures where no other technique can access such
Seeger and Chick [Seeger68] were the first to suggest that the mono-vacancies in silicon
and germanium behaved differently. They suggested that the mono-vacancy in germanium
was a point defect whereas the mono-vacancy in silicon was an extended defect, i.e. many Si
atoms sharing the vacancy causing different diffusion behaviour at elevated temperatures.
Bracht et al. [Bracht03], gave experimental evidence that the diffusivity of the mono-vacancy
in Si at elevated temperatures (between 780°C and 872°C) occurs with much higher
activation energy (1.7(5) eV), than observed at low temperatures (0.25-0.45 eV [Watkins91]).
It was suggested that this behaviour is related to the extended nature of the vacancy at
elevated temperatures, but their results are disputed [Suezawa08, Watkins08].
The hypothesis of a slow vacancy (high activation energy) at elevated temperatures has
been supported by Mössbauer investigations at ISOLDE, using implantation of 57 Mn
[Gunnlaugsson03, Weyer07], but further investigations are needed in order to substantiate
The diffusivity of the (uncharged) mono-vacancy in silicon is outlined in the Arrhenius plot
in Fig. 5.
Log 10(D V (cm 2 /s))
Bracht et al., 2003
Voronkov and Falser, 2009
Current interpr. of ISOLDE data
1.2×10 -3 exp(-0.45 eV/kT) cm 2 /s
0 1 2 3 4 5 6 7 8
1000/T (K -1 )
Fig. 5: Arrhenius plot showing the diffusivity of the mono-vacancy in silicon
Watkins et al. [Watkins91] found the mono-vacancy to behave as a point defect at cryogenic
temperatures where it is thermally stable. Extrapolating his data to temperatures close to the
melting temperature coincides with the data from Voronkov and Falster [Voronkov09] based
on growth properties. Bracht et al., [Bracht03] did not determine the exponential pre-factor of
the diffusion but determined the activation energy (slope) to be much higher.
This is where we have the possibility to obtain unique data using implantation of 57 Mn for
57 Fe Mössbauer spectroscopy. Upon implantation and annealing of the implantation damage
(~400 K) [Weyer03, Gunnlaugsson02b], the Mn probe is predominantly on substitutional
sites and as MnI-V complexes, based on preliminary analysis of EC experiments [Wahl11]. In
the recoil, a sizeable fraction of the Mn atoms is expelled into interstitial sites
[Gunnlaugsson02a], creating a vacancy nearby. If the vacancy follows the mobility assumed
by extrapolation of the Watkins data (dashed line in Fig. 5), one would expect the
recombination of the interstitial Fe atom and the vacancy between 350–400 K. However, this
recombination is only observed at 600–650 K, suggesting a “slow” vacancy. Moreover, the
interstitial Fe atom does not jump into the vacancy to form substitutional Fe, but forms a
metastable pair, possibly due to the extended nature of the vacancy [Seeger68].
It is unlikely that it is the presence of the interstitial Fe atom that affects the configuration
of the vacancy in silicon. In SiGe (unpublished data from the IS426 experiment, awaiting
more detailed data from current experiment), we observe a transition from a “slow” vacancy
in Si1-xGex for x < 0.1 to a “fast” vacancy for x > 0.25.
The basic tools used by us, are temperature mapping and so-called time-delayed
measurements (TDM) [Gunnlaugsson09] using 57 Mn. The temperature mapping allows us to
make a firm identification of (overlapping) spectral components (position in spectra,
quadrupole splitting, line-width, Debye temperatures) due to the different in-growth and
disappearance of spectral components as a function of temperature. As the behaviour of some
of the spectral components differs between materials, cross correlation of spectral parameters
between different types of materials will make this identification stronger (the aim of the
current proposal). In TDM we implant for relatively short time (~100 s) and follow the fate of
spectral components as a function of time during the 1.5 minutes lifetime of 57 Mn. This
allows us to distinguish whether the spectral components are formed during the lifetime of
the 57 Mn (~minutes) or during the lifetime of the Mössbauer state of 57 Fe (100’s of ns). As
the TDM’s need to be repeated to obtain sufficient statistics, we also get information on
potential fluence dependence.
The status of our measurement plan is outlined in Fig. 6.
Beam times Temperature mapping (K)
Recorded data Unrecorded data Silicon material
2 Ratio of MnS/MnI(-
3 What is near
formation is not
In MS we
ideal T site,
while in EC it
is shifted from
the ideal T site
4 Assignment of FeS-V Currently very
5 Formation of FeS-V Why is FeS-V
6 Outdiffusion of
3.3.1 119 In
Should lead to
lines in MS,
~800 K of
observations are at 600
MnI forms a complex
with vacancy. With a
binding energy ~1 eV,
it dissociates in the
recoil and FeI is
observed as ideal
Dissociation of VO
Formed, but dissociated
due to the recoil? Not
in the temperature
range from 300-500
EC at low
measurements at T’s
where V is immobile
should give the ideal
in FZ and HP
Comparison of MS
results in all types of
materials + EC at
on EC on 57 Mn at T
= 750-850 K or
56 Mn, MS
high temperatures in
n ++ Si
In 2010, we attempted to apply 119 In (T½ = 2.1 min) for 119 Sn Mössbauer spectroscopy.
Among the aims was to apply TDM’s to observe the formation of In-V pairs. Such pairs have
been observed in 111 In PAC studies [Deicher87]. Surprisingly, the analysis of the data did not
require the presence of a In/Sn-V component. A possible explanation for this is that it is too
small to be observed, or that the parameters of such a component are too similar to the
substitutional Sn to be distinguished from it with the statistics that were available.
To obtain a complete picture of the group IV semiconductors, implantations into diamond,
SiGe and Ge were also performed in 2010. Fig. 7 summarizes some of the findings.
C SiC Si Ge -Sn
1,2 119mSn and
1,5 2,0 2,5 3,0
Bond length (Å)
Fig. 7: Isomer-shifts of damage sites and in substitutional sites in diamond-type lattices of group IV
While SiC – -Sn shows the expected pressure dependence of the isomer-shift for the
substitutional line, there is an apparent jump for diamond (C). This is possibly due to the
large size of the Sn atom, not being able to enter a simple substitutional site, and may be
related to the same effect as observed in oxide semiconductors described in section 2.2. In
2010 we had only small diamond samples and were unable to get useful Mössbauer signal
(which is strange in view of the fact that diamond has the highest Debye Waller factor of the
group IV semiconductors). In 2011 we had a large area CVD diamond sample, characterized
the annealing reactions with 57 Mn implantations, but the 119 In beam was too poor to allow for
this data to be taken.
3.4 Experimental plan
The data taking for the tasks labeled as “very important” and most of the “important”
outlined in Fig. 6 is estimated to take ~32 hours (~4 shifts) and this would cover items 4 and
part of items 5 and 6 outlined in Table 1. The time needed for performing emission
channeling on 57 Mn is based on experience from 2011 (items 2, 3 and part of 5 & 6). Here it
was found that measurement at single temperature takes ~2 hours, so full mapping of two
different types of samples is estimated to need ~24 hours (=3 shifts) [Wahl11]. The EC
dataset obtained using 57 Mn (T½ = 1.5 min) will also help in the interpretation of the dataset
obtained using RT implantation and annealing experiments with the longer-lived 56 Mn (T½ =
2.6 h) which is a part of the IS453 experiment [Wahl11]. It should be noted here that the
short-lived Mn is essential if one wants to study the lattice location
of Mn as a function of implantation temperature. Such experiments cannot be performed
with 56 Mn in reasonable time since after each implantation and measurement step one would
have to wait about 6 h until the old activity has decayed and a new implantation at a different
temperature can take place.
With laser ionization of In, it should be possible to further apply TDM’s in silicon to see
whether In-V pairs form, and in that case investigate this capture of vacancies further, and to
complete the picture of group IV semiconductors by temperature mapping in CVD diamond.
One shift should be sufficient for this. This data could be supported by 119m Sn implanted
samples, where less than a whole shift would be sufficient.
4 Experimental and samples
4.1 Mössbauer spectroscopy
The Mössbauer collaboration has a multi-purpose implantation chamber to perform on-line
experiments (cf. Fig. 8).
Fig. 8: Picture of the implantation chamber used for Mössbauer measurements of short lived isotopes in
configuration used for elevated temperatures. The sample holder is attached to the lid and different lids
are used for the different applications.
Different experimental conditions (temperature, rotation, external magnetic field) are
installed by placing different types of lid’s onto the chamber. Some of these facilitate up to 4
samples in the same load. With new pumps, sample change takes of the order 15 minutes. For
the experiments we have detectors with 57 Fe enriched stainless steel electrodes and for the
2012 beam time a newly developed 57 FeAl detectors which we expect (hope) will increase the
counting effect by factor 2.
The Mössbauer collaboration counts currently 16 researchers from 9 institutes (cf.
Appendix 3). On the average 10-14 persons are active in data taking during the on-line
experiments, ensuring enough manpower.
4.2 Emission channelling
The emission channelling group is led by U. Wahl. They have on-line chamber for
performing emission channelling on short lived isotopes. During the 2011 beam time, a test
using 57 Mn was performed and was successful. It was seen that sufficient data under single
emission angle was obtained in ~40 minutes. Full measurement at single temperature (3
emission angles) takes ~2 hours, and these numbers have been used as the input in the beam
To illustrate the usefulness of 57 Mn for emission channeling, Fig. 9 shows the emission
patterns obtained from room temperature implantation of 57 Mn in to n-type Si.
Fig. 9: Emission channeling and best fit, assuming substitutional site (S) and displaced tetrahedral
interstitial site (T) [Wahl11]. Note there is a higher background toward the lower-left in the experimental
The fractions found are 12(2)% at S sites + 8(2)% displaced 0.4(2) Å from the ideal T-site.
These fractions have not yet been background corrected, but illustrate that despite the
relatively high electron energy that 57 Mn is a good EC isotope.
4.3 Perturbed Angular Correlation
It is possible to perform e - — Perturbed Angular Correlations (PAC) experiments on 119m Sn
[Soares73]. It is an excellent PAC 3/2 isotope where K or L conversion electrons from the
first transition are used for triggering the start while the M1 ray used in Mössbauer
experiments triggers the stop. A Siegbahn-type spectrometer, providing measurements from
30 K up to 800 K, is in operation at ISOLDE and is the ideal setup for performing such
measurements. Samples would be prepared for both PAC and Mössbauer spectroscopy,
allowing for direct comparison between the results obtained by both techniques.
Measurement times are similar as with Mössbauer spectroscopy (~weeks). In case that the
Mössbauer results are complicated, PAC may give complementary information on their
interpretation by determining values of the quadrupole interaction. Decisions on which
samples would be potentially used for PAC will be taken on the basis of the Mössbauer
4.4 Theoretical calculations
Our identification of defects can be supported by theoretical calculations of hyperfine
parameters. We collaborate with A. Svane at the Aarhus University in this respect. He applies
quantum mechanical calculations based on the local density approximation to density
functional theory on a supercell with Fe or Sn atoms. The calculations give information on
total energies and Mössbauer hyperfine parameters. Currently Svane is working on (among
(1) Calculations of isomer-shifts of substitutional Sn in diamond and Sn in a di-vacancy
in diamond. This will become relevant in the interpretation of the “jump” shown in
(2) Calculations of isomer-shifts of Sn in oxides and II-VI’s. This is motivated by the
observation of Sn 4+ instead of Sn 2+ in several oxides following implantation of 119 In.
In some of the II-VI’s (e.g. ZnSe) the covalent nature of the bindings result in isomershifts
that are not necessarily directly characteristic for the charge state of the Sn
atom, and only with the aid of theoretical calculations one can come to firm
(3) Calculations of hyperfine parameters and properties of Fe in silicon. At the moment
we have only very tentative identification of the FeS-V complex, and this hypothesis
can be supported or rejected by the results of theoretical calculations.
We have access to all sample types discussed in our proposal, in particular different types of
Cz silicon single crystals from collaboration with the semiconductor group of Arne
Nylandsted Larsen at Aarhus University in Denmark, were we also have access to moderately
doped float-zone (FZ) grown material and some higher doped high purity (HP) MBE grown
material. Oxides and selected II-VI’s are available commercially and large area CVD
diamond sample is available.
5 Summary of requested shifts
First, here is a list of how we intend to use the beam time (if awarded)
1. Paramagnetic relaxations in
2a. Vacancy diffusion in Si
2 1.6 3 6.6
based semiconductors 4 1 0.75 5.75
2b. Vacancy diffusion in Si
based semiconductors 3 3
(Emission channelling shifts)
Calibration (~10%) 0.25 0.15 0.4
0.25 0.5 0.5 0.25 0.25 1.25
Total 9.5 0.5 2.75 4 0.25 17
Only used if other users are requesting suitable target/beam
This totals to 9.25 on-line Mössbauer shifts ( 57 Mn and 119 In), which is similar to the shifts we
have been able to use per year. Implantation of the other isotopes does not require the same
manpower, as the Mössbauer measurements are performed off-line at home laboratories or at
We request additional beam-time for contingency/opportunistic science. We often get
requests for measurements of high scientific value, that require only 1-2 hour of beam-time.
Such experiments have previously resulted in new proposals or allowed us to demonstrate
that the physics program is feasible. In 2011, this addition was very important due to the low
intensity of the beam and allowed us to get data for the main subjects of the proposal.
Table 2: Formal beam request.
Energy Shifts Target Ion source Desired Proton
≥ 50 9.5 UCx Mn RILIS 2 A
(270 d) b
VADIS/RILIS(?) 2 A(at
In (2.1 (2-3)×10
≥ 50 2.75 UCx In RILIS 2 A
≥ 50 4 UCx Sn RILIS 2 A
≥ 50 0.25
UCx Sb RILIS 2 A
For the Mössbauer part. > 0.5 µA for the Emission channelling part
We take all nuclei that eventually decay to 57 Co. Note, 57 Co builds up within ZrO2 or YO
targets. By keeping these targets cold during proton irradiation enables long-lived 57 Co to be
extracted by heating the target unit. Protons are not necessarily needed at this stage.
c Impurities should be below ~10%, Tellurium impurities ( 119 Te (T½ = 4.7 d) have to be
d If suitable beam is provided for other purpose
5.1 Beam details
For all the isotopes, and especially the Mössbauer part of 57 Mn, it is requested that as close to
2 A of proton current be delivered as is possible. These runs should be dedicated to GPS
only. Unlike some solid state runs, sharing with HRS in parallel is not feasible and results in
lower yields (as in 2011).
5.1.1 57 Mn (T½ = 1.5 min.)
This is the beam the group is very familiar working with. The measurements are done online
in the setup described in section 4.1. Our experience for the last many years is that we use
roughly 5-6 shifts per year of 57 Mn assuming “normal” intensities (~2×10 8 57 Mn/s). In 2011,
the intensity was much lower (see section 8).
5.1.2 57 Co (T½ = 270 d)
57 Co is of high interest for the Mössbauer collaboration as the number of facilities offering
this beam has decreased significantly since the 90’s. Unfortunately, the current beam
provided at ISOLDE has high 57 Fe impurities to be well useful in all context. Experience
from 2010 and 2011 (YtO2 target and VADIS ion source) tells us that with optimum settings
a weak source can be produced in half shift.
In principle, a RILIS scheme exists for Co beams, which would reduce the Fe impurities
which have caused problems with these beams over the last couple of years. Although
unlikely to be used during a “normal” ZrO2 or YO run, this could potentially be employed at
the end of the running period in 2012, if long-lived isotopes are being delivered instead of the
usual separator courses. As mentioned above, protons would not be needed if the target had
been already irradiated, but kept cold.
Implanted samples would then be shipped to home institutes.
5.1.3 119 Sb (T½ = 38 h)
Due to the lifetime the samples should be implanted, and taken for measurements and
annealing at ISOLDE. Recent technical additions, at the solid state laboratory at ISOLDE,
make this a favorable way of doing the measurements. Chambers for making measurements
at low temperatures exist in Aarhus and will be transported to ISOLDE, and either the on-line
chamber or a new chamber will be used for measurements at temperatures above room
temperature. We do not consider us a major user of such a beam, but if it is provided, we
would like to have half shift for testing and obtaining data for comparison with other
119 Sb can be produced with an UCx target and a Sb RILIS ion source. 119 In impurities
decay quickly and will not disturb the measurements. About 4×10 8 /µC for 119 Sb are estimated
Another possibility is using a LaCx target and a MK5 ion source, but this will produce
more 119 Te, which has a half live of 4.7 days and would therefore hamper studying the Sb
behavior in the systems we are interested in [Koster09].
5.1.4 119m Sn (T½ = 290 d)
Implantations would be performed at ISOLDE and measurements and annealing in home
laboratories. As of yet, we have not been requesting this beam for the IS501 experiment, but
at this stage it is feasible in order to get data during the 2013 shutdown.
119m Sn can be produced with an UCx target and a Sn RILIS ion source. Yields of 119 Sn
have been measured 1.8×10 9 /µC [Koster08]. Both the 119g Sn and 119m Sn are produced, but
1.0×10 9 /µC of 119m Sn can be expected with some background of 119 Cs and 119 In, but not at a
disturbing level [Koster09].
Molecular beams are not suitable for our measurements.
Production with LaCx target and Sn RILIS ion source is a possibility with yield of ~
1.3×10 7 /µC of 119m Sn [Koster09]. This, however, requires much longer implantation time, but
would be an option to prepare a weak source if the implantation can be done parallel with
other experiments and the UCx target and Sn RILIS is not available [Koster09].
5.1.5 119 In (T½ = 2.1 min)
119 In has a very similar half live as 57 Mn, and the same setup is used. In 2010 we had UCx
and Ta/W surface ion sources that gave ~ 4×10 7 /µC, which is on the borderline of what is
feasible, and does not allow for TDM’s. The laser ionization scheme is fairly simple (one
resonance and ionization) [Koster11] and should be possible to set up quickly. Assuming that
this gives a factor of 3 compared to W surface ionizer, the yields are estimated to 1.3×10 8 /µC.
5.2 Sample preparation
For the long lived isotopes ( 57 Co and 119m Sn) experience (G. Weyer, private communication)
is that a source strength of ~0.1 MBq (~3 µCi) is the minimum required for having a useful
source to use in the laboratory (10-20 measurements of sufficient quality during 1 year).
In the case of 119m Sn the beam quality at ISOLDE allows us to request a good source
strength (0.6 MBq, ~15 µCi), with a total dose just below where the transition threshold from
amorphous pockets to amorphous layers (around 5×10 13 cm -2 , see e.g. [Weyer82]). With the
beam estimates it will be possible to produce two such samples per shift.
For 119 Sb, we estimate that for a single implantation, we should have a starting activity of
about 370 MBq (10 mCi), which is enough to perform ~10 good measurements within ~70
hours. This requires ~7.3×10 12 atoms implanted, and is well below the amorphization limit.
With the above estimate of ~4×10 8 /µC 119 Sb/s, the making a suitable sample takes of the
order of 3-4 hours allowing the preparation of two samples per shift.
[Bracht03] H. Bracht, J. Fage Pedersen, N. Zangenberg, A. Nylandsted Larsen, E. E. Haller,
G. Lulli and M. Posselt, Radiation Enhanced Silicon Self-Diffusion and the
Silicon Vacancy at High Temperatures, Phys. Rev. Lett. 91 (2003) 245502, doi:
[Dietl00] T. Dietl, H. Ohno, F. Matsukura, J. Cibert and D. Ferrand, Zener Model
Description of Ferromagnetism in Zinc-Blende Magnetic Semiconductors,
Science 287 (2000) 1019-1022, doi: 10.1126/science.287.5455.1019
[Deicher87] M. Deicher, G. Grübel, E. Recknagel, H. Skudlik and Th. Wichert, Structural
lattice defects in silicon observed at 111 In by perturbated angular correlation,
Hyp. Int. 35 (1987) 719-722
[Gunnlaugsson02a] H. P. Gunnlaugsson, G. Weyer, M. Dietrich, the ISOLDE
collaboration, M. Fanciulli, K. Bharuth-Ram and R. Sielemann, Charge state
dependence of the diffusivity of interstitial Fe in silicon detected by Mössbauer
spectroscopy, Appl. Phys. Lett. 80 (2002) 2657-2659, 10.1063/1.1469216.
[Gunnlaugsson02b] H. P. Gunnlaugsson, M. Fanciulli, M. Dietrich, K. Baruth-Ram, R.
Sielemann, G. Weyer and the ISOLDE collaboration. 57 Fe Mössbauer study of
radiation damage in ion implanted Si, SiGe and SiSn, Nucl. Inst. Meth. B,
168(1-4) (2002) 55-60.
[Gunnlaugsson03] H. P. Gunnlaugsson, G. Weyer, N.E. Christensen, M. Dietrich, M.
Fanciulli, K. Bharuth-Ram, R. Sielemann, A. Svane, and the ISOLDE
Collaboration, On the kinetics of the formation of interstitial Fe-vacancy pairs at
high temperatures, (2003) Physica B, 340-342 (2003) 532-536, doi:
[Gunnlaugsson09] H. P. Gunnlaugsson, G. Weyer, R. Mantovan, D. Naidoo, R.
Sielemann, K. Bharuth-Ram, M. Fanciulli, K. Johnston, S. Olafsson, G.
Langouche, Isothermal defect annealing in semiconductors investigated by timedelayed
Mössbauer spectroscopy: Application to ZnO, Hyp. Int. 188 (2009) 85–
89, doi: 10.1007/s10751-008-9893-4.
[Gunnlaugsson10a] H. P. Gunnlaugsson, T. E. Mølholt, R. Mantovan, H. Masenda, D.
Naidoo, W. B. Dlamini, R. Sielemann, K. Bharuth-Ram, G. Weyer, K. Johnston,
G. Langouche S. Ólafsson, H. P. Gíslason, Y. Kobayashi, Y. Yoshida, M.
Fanciulli and the ISOLDE Collaboration, Paramagnetism in Mn/Fe implanted
ZnO, Appl. Phys. Lett. 97 (2010) 142501, doi:10.1063/1.3490708
[Gunnlaugsson10b] H.P. Gunnlaugsson, R. Mantovan, T.E. Mølholt, D. Naidoo, K.
Johnston, H. Masenda, K. Bharuth-Ram, G. Langouche, S. Ólafsson, R.
Sielemann, G. Weyer, Y. Kobayashi and the ISOLDE Collaboration,
Mössbauer spectroscopy of 57 Fe in α-Al2O3 following implantation of 57 Mn * ,
Hyp. Int. 198 (2010) 5-14
[Gunnlaugsson10c] H. P. Gunnlaugsson, R. Sielemann, T.E. Mølholt, W.B. Dlamini, K.
Johnston, R. Mantovan, H. Masenda, D. Naidoo, W.N. Sibanda, K. Bharuth-
Ram, M. Fanciulli, H.P. Gíslason, G. Langouche, S. Ólafsson, G. Weyer and the
ISOLDE Collaboration, Magnetism in iron implanted oxides: a status report,
Hyp. Int. 197 (2010) 43-52
[Gunnlaugsson12a] H. P. Gunnlaugsson, K. Johnston, T. E. Mølholt, G. Weyer, R.
Mantovan, H. Masenda, D. Naidoo, S. Ólafsson, K. Bharuth-Ram, H. P.
Gíslason, G. Langouche, M. B. Madsen and the ISOLDE Collaboration, Lattice
locations and properties of Fe in Co/Fe co-implanted ZnO, Appl. Phys. Lett.
[Gunnlaugsson12b] H. P. Gunnlaugsson et al., Implantation damage in ZnO (working
[Istratov99] A. A. Istratov, H. Hieslmair, E. R.Weber, Iron and its complexes in silicon,
Appl. Phys. A 69 (1999) 13–44, doi: 10.1007/s003399900059
[Jung02] S. W. Jung, S.-J. An, Gyu-Chul Yi, C. U. Jung, Sung-Ik Lee, and S. Cho,
Ferromagnetic properties of Zn1–xMnxO epitaxial thin films, Appl. Phys. Lett. 80
(2002) 4561, doi:10.1063/1.1487927.
[Kapilashrami09] M. Kapilashrami, J. Xu, V. Ström, K. V. Rao, and L. Belova1, Appl.
Phys. Lett. 95, 033104 (2009), doi: 10.1063/1.3180708.
[Khalid09] M. Khalid, M. Ziese, A. Setzer, P. Esquinazi, M. Lorenz, H. Hochmuth, M.
Grundmann, D. Spemann, T. Butz, G. Brauer, W. Anwand, G. Fischer, W. A.
Adeagbo, W. Hergert, and A. Ernst, Phys. Rev. B 80, 035331 (2009), doi:
[Koji06] A. Koji, Seeking Room-Temperature Ferromagnetic Semiconductors, Science
312 (2006) 1883, DOI: 10.1126/science.1125461.
[Koster08] U. Köster, O. Arndt, E. Bouquerel, V. N. Fedoseyev, H. Frånberg, A. Joinet, C.
Jost, I. S. K. Kerkines, R. Kirchner, the TARGISOL Collaboration, Progress in
ISOL target–ion source systems , Nucl. Instr. Meth. B 266 (2008) 4229–4239,
[Koster09] Ulli Köster, Private communication, 2009
[Koster11] Ulli Köster, Private communication, 2011
[Kucheyev03] S. O. Kucheyev, C. Jagadish, J. S. Williams, P. N. K. Deenapanray, Mitsuaki
Yano, Kazuto Koike, Shigehiko Sasa, Masataka Inoue, and Ken-ichi Ogata,
Implant isolation of ZnO, J. Appl. Phys. 93, 2972 (2003),
[Mantovan12] R. Mantovan, H. P. Gunnlaugsson, D. Naidoo, S. Ólafsson, T. E. Mølholt, K.
Johnston, K. Bharuth-Ram, M. Fanciulli, G. Langouche, R. Sielemann, G.
Weyer, H. P. Gíslason, M. B. Madsen and the ISOLDE Collaboration, Fe charge
state tuning in ZnO upon ion implantation, (2012) In prep.
[MossbColl] Mössbauer collaboration at ISOLDE/CERN web pages (preliminary as of
January 2012) http://phys.au.dk/forskning/moessbauer-collaboration-atisoldecern/.
Here one can find updated list of publications and presentations at
[Mølholt09] T. E. Mølholt, R. Mantovan, H. P. Gunnlaugsson, K. Bharuth-Ram, M.
Fanciulli, H. P. Gíslason, K. Johnston, Y. Kobayashi, G. Langouche, H.
Masenda, D. Naidoo, S. Ólafsson, R. Sielemann and G. Weyer, Temperature
and dose dependence of defect complex formation with ion-implanted Mn/Fe in
ZnO, Physica B 404 (2009) 4820-4822, doi: 10.1016/j.physb.2009.08.187.
[Mølholt10] T.E. Mølholt, R. Mantovan, H.P. Gunnlaugsson, D. Naidoo, S. Ólafsson, K.
Bharuth-Ram, M. Fanciulli, K. Johnston, Y. Kobayashi, G. Langouche, H.
Masenda, R. Sielemann, G. Weyer and H.P. Gíslason, Observation of spinlattice
relaxations of dilute Fe 3+ in MgO by Mössbauer spectroscopy, Hyp. Int.
197 (2010) 89-94
[Mølholt12] T. E Mølholt, H. P. Gunnlaugsson, K Johnston, R. Mantovan, H. Masenda, S.
Ólafsson, K. Bharuth-Ram, H. P. Gislason, G. Langouche, G. Weyer and the
ISOLDE Collaboration, Spin-lattice relaxations of paramagnetic Fe 3+ in ZnO,
Physica Scripta (2012) Accepted for publication.
[Naidoo12] D. Naidoo et al., Annealing of Fe 3+ state in ZnO (working title), TBD
[Osgur05] Ü. Özgür, Ya. I. Alivov, C. Liu, A. Teke, M. A. Reshchikov, S. Doğan, V.
Avrutin, S.-J. Cho and H. Morkoç, A comprehensive review of ZnO materials
and devices, J. Appl. Phys. 98 (2005) 041301, DOI: 10.1063/1.1992666.
[Potzger06] K. Potzger, Shengqiang Zhou, H. Reuther, A. Mücklich, F. Eichhorn, N. Schell,
W. Skorupa, M. Helm, J. Fassbender, T. Herrmannsdörfer, T. P. Papageorgiou,
Fe implanted ferromagnetic ZnO, Appl. Phys. Lett. 88 (2006) 052508;
[Potzger09] K. Potzger, and S. Zhou, Non-DMS related ferromagnetism in transition metal
doped zinc oxide, Phys. Status Solidi B 246 (2009) 1147-1167, doi:
[Seeger68] A. Seeger and K. P. Chik, Diffusion Mechanisms and Point Defects in Silicon
and Germanium, Phys. Status Solidi B 29 (1968) 455-542, doi:
[Soares73] J. C. Soares, K. Krien, A. G. Bibiloni, K. Freitag and R. Vianden, Determination
of the quadrupole splitting of the first excited state of 119 Sn in -tin by the e - –
TDPAC technique, Phys. Lett. A, 45 (1973) 465-466, doi:10.1016/0375-
[Suezawa08] M. Suezawa and I. Yonenaga, On the Extended Point Defect Model in Si
Crystals at High Temperature, Jpn. J. Appl. Phys. 47 (2008) 7117–7118, doi:
[Srivastava80] K. K. P. Srivastava and S. N. Mishra, Dynamic Spin Hamiltonian Formalism
and Mössbauer Study of Spin—Lattice Relaxation of Paramagnetic Fe 3+ ( 6 S)
Ions, Phys. Status Solidi b 100 (1980) 65-75, DOI: 10.1002/pssb.2221000105
[Ye09] H. B. Ye, J. F. Kong, W. Pan, W. Z. Shen, B. Wang, Multi-carrier transport
properties in p-type ZnO thin films, Solid State Comm. 149 (2009) 1628-1632,
[Voronkov09] V.V. Voronkov, R. Falster, Gigantic uphill drift of vacancies and selfinterstitials
in silicon, Mat. Sci. Eng. B, 159-160 (2009) 138-141, DOI:
[Wahl05] U. Wahl, J. G. Correia, E. Rita, J. P. Araújo, J. C. Soares, The ISOLDE
Collaboration, Lattice sites of implanted Fe in Si, Phys. Rev. B, 72 (2005)
[Wahl06] U. Wahl, J. G. Correia, E. Rita, J. P. Araújo, J. C. Soares, The ISOLDE
Collaboration, Fe and Cu in Si: Lattice sites and trapping at implantation-related
defects, Nucl. Instr. Meth. B 253 (2006) 167–171
[Wahl11] U. Wahl, private communications based on preliminary analysis of 57 Mn
emission channelling data of 57 Mn from 2011.
[Wang08] Q. Wang, Q. Sun, G. Chen, Y. Kawazoe and P. Jena, Vacancy-induced
magnetism in ZnO thin films and nanowires, Phys. Rev. B 77 (2008) 205411,
[Wang09] Q. Wang, Q. Sun, P. Jena, and Y. Kawazoe, Magnetic properties of transitionmetal-doped
Zn1−xTxO (T=Cr, Mn, Fe, Co, and Ni) thin films with and without
intrinsic defects: A density functional study, Phys. Rev. B 79, (2009) 115407,
[Watkins91] G.D. Watkins, in: W. Schröter (Ed.), Materials Science and Technology, Vol. 4,
VCH, Weinheim, 1991, p. 105.
[Watkins08] G. D. Watkins, The vacancy in silicon: Identical diffusion properties at
cryogenic and elevated temperatures, J. Appl. Phys. 103 (2008) 106106, doi:
[Weyer80a] G. Weyer, S. Damgaard, J. W. Petersen, J. Heinemeier, Mössbauer study of
119 Sn defects in silicon from ion implantations of radioactive 119 In, Hyp. Int. 7
(1980) 449-453, doi: 10.1007/BF01021527.
[Weyer80b] G. Weyer, A. Nylandsted Larsen, N. E. Holm, H. L. Nielsen, Radiation defects
in ion-implanted silicon. I. Mössbauer spectrsocopy of 119 Sn defect structures
from implantation of radioactive antimony, Phys. Rev. B 21 (1980) 4939-4950,
[Weyer80c] G. Weyer, S. Damgaard, J. W. Petersen, J. Heinemeier, Sn impurity defects in
germanium from ion implantations of radioactive 119 In, Phys. Lett. 76A (1980)
321-323, doi: 10.1016/0375-9601(80)90506-X.
[Weyer82] G. Weyer, S. Damgaard, J. W. Petersen, J. Heinemeier, Comparison of Impurity
Defect Structures Formed By Ion Implantation In Amorphous and Crystalline
Silicon, Nucl. Instr. Meth. 199 (1982) 441-444, doi: 10.1016/0167-
[Weyer99] G. Weyer, A. Burchard, M. Faciulli, V. N. Dedoseyev, H. P. Gunnlaugsson, V.
I. Mishin, R. Sielemann, The ISOLDE Collaboration, UThe electronic
configuration of substitutional Fe in silicon U, Phys. B, 273-274 (1999) 363-366.
[Weyer03] G. Weyer, H. P. Gunnlaugsson, M. Dietrich, M. Fanciulli, K. Baruth-Ram, R.
Sielemann and the ISOLDE collaboration. Creation and annealing of defect
structures in silicon-based semiconductors during and after implantation at 77-
500 K, Nucl. Instr. Meth. B, 206 (2003) 90-94, doi: 10.1016/S0168-
[Weyer07] G. Weyer, Defects in semiconductors-results from Mössbauer spectroscopy,
Hyp. Int. 177 (2007) 1-13, doi: 10.1007/s10751-008-9607-y
[Zhou09] S. Zhou, K. Potzger, Q. Xu, G. Talut, M. Lorenz, W. Skorupa, M. Helm, J.
Fassbender, M. Grundmann, H. Schmidt, Ferromagnetic transition metal
implanted ZnO: A diluted magnetic semiconductor? Vacuum 83, S13 (2009),
7 Appendix 1: The Mössbauer collaboration at
Our team, which initially called itself “The Mn Mössbauer collaboration at
ISOLDE/CERN” has grown significantly in recent years, and now consist of 14 members
directly involved in the Mössbauer measurements. Nine of the members 9 have expertise in
running the equipment and the measurements. Hence, we will be able to make use of an
increased number of beams, expanding considerably the range and depth of the scientific
questions that can be addressed.
The list below contains the members and the most important collaborating partners with
respect of the current proposal.
More details can be found on the group web pages (http://phys.au.dk/forskning/moessbauercollaboration-at-isoldecern/
[MossbColl]). Note that these pages are incomplete at present,
but are expected to be advertised in 2012 on completion.
Country/Institutions Members Facilities
Denmark, Department of
Physics and astronomy,
Iceland, Science Institute,
University of Iceland.
Italy, CNR-IMM MDM
Laboratory, Via C. Olivetti
2, 20041 Agrate Brianza
South Africa, School of
Physics, University of the
of KwaZulu-Natal, Durban;
iThemba LABS, Somerset
Belgium, Instituut voor
Kern-en Stralings fysika,
University of Leuven.
Switzerland, EP Division,
H. P. Gunnlaugsson, G.
S. Ólafsson, H. P. Gíslason,
T. E. Mølholt (PhD student)
Mössbauer Lab., theoretical
calculations of Mössbauer
hyperfine parameters (A.
Mössbauer Lab., Sputtering
growth of various samples,
with various types of
R. Manotvan Mössbauer Lab. Growth of
samples (ALD) and various
D. Naidoo, K. Bharuth-
Ram, M. Moodley, H.
Masenda (PhD student), M.
Ncube (PhD student)
Mössbauer Labs., Ion beam
analysis and Magnetization
Specialists in Hyperfine
Interactions and Nuclear
Methods in Solid State
G. Langouche Mössbauer Lab., Specialist
in Mössbauer spectroscopy
K. Johnston Radioactive Laboratory,
equipment for annealing
and off-line Mössbauer
J. G. Correia (PAC) U.
Contact persons regarding
PAC and EC experiments
Tecnológico e Nuclear
(ITN), Sacavém; IFIMUP,
Porto; Centro de Fisica
Nuclear da Universidade de
Lisboa (CFNUL), Lisboa
Denmark, Niels Bohr
Institute, University of
France, IM2NP, Aix- ,
overlapping with the IS481
M. B. Madsen Mössbauer Lab., Specialist
on relaxation phenomena
A. Mesli Specialist on metal defects
8 Appendix 2: Beam reports 2010&2011
In the following, some relevant information from beam reports from the IS501 experiment
are summarized. As the request for opportunistic science may be unorthodox, we have
included a description of how that was used and the main outcome.
57 Co (T½ = 271 d): Very high impurity level of 57 Fe (~99% of the beam). Limits
considerably the application range for this beam for our purposes. Still one sample
prepared where the impurity level was beneficial for the interpretations
Mn (T½ = 1.5 min): Very successful, with intensity ~2×10 8 ions/s. Used up the shifts
from the IS443 experiment and started on the new IS501 experiment. Implantation
energy had to be limited to 40 keV, which proved useful. Some strange results
obtained during this beam-time were repeated in 2011 (50 keV beam) and were not
reproducible, meaning that we maintain the wish for ≥ 50 keV beam.
In, no. 1 (T½ = 2.1 min): Failed due to target failure. We were able to demonstrate
that our detector system worked.
119 In, no. 2 (T½ = 2.1 min): Unexpected low intensity (~2×10 7 ions/s) limiting the
usefulness of this beam. Surprising in view of intensities ~10 9 ions/s in the 80’s
[Weyer80-Weyer82]. Still good data acquired, but some experiments impossible.
RILIS ionization requested in this addendum.
Co (T½ = 271 d): Low intensities and few very weak sources prepared. Still high
impurity level of 57 Fe (~99% of the beam).
Mn (T½ = 1.5 min): Unusually low intensity ~7×10 7 ions/s. Extension of the beam
time helped in getting our data of high importance. Some data shows unexpected dose
dependence, and this is probably due to unusually small beam-spot due to unusually
well focused beam [Johnston11]. Clearly we need to make a short implantation of
longer lived isotope (e.g. 56 Mn) in order to document the size and distribution of the
beam-spot. Low intensity of the beam partly due to sharing of the beam with HRS
experiment. For the Mössbauer part of 57 Mn this is not feasible and results in
compromised beamtimes. Optimal conditions for production of 57 Mn are with as close
to 2 µA of protons as possible.
In (T½ = 2.1 min): Only one measurement performed, intensity estimated to be
Vacancy diffusion in group IV
Opportunistic science 5%
The low intensity of the 57 Mn/ 119 In beams in 2011 meant that almost no opportunistic science
was performed. As only very minor changes were made to the experimental setup, calibration
tasks were simple. With a new detector for 57 Fe in 2012, some additional calibration has to be
performed. The main opportunistic science 2010-2011 is outlined in Table 4.
Table 4: Main opportunistic science in 2010 and 2011
57 Mn for
Implantation damage does not destroy the superlattice.
Publication being prepared [Mølholt et al.]. Could
result in a proposal/Lettor of intent after 2013.
Helps in interpretation of data from GaN, so only
partly opportunistic science. Should result in
publication [Masenda et al.]
Test performed with 57 Mn ( 119 In scheduled for 2011
and cancelled). Major changes during phase change
observed, inconsistent with some of the literature. Data
being analyzed, and could result in a proposal after
2013 [Mantovan et al.,]
Test of 57 Mn for Emission channeling experiments.
Despite high electron energies, good results were
obtained, illustrating the usefulness of this isotope
Other opportunistic science tasks that were on our plan in 2011 were cancelled and the beam
time used for obtaining the data for the proposal. This included temperature mapping in Ar
implanted ZnO [Bharuth-Ram et al.,], search for Fe-Fe dimer in Si [Langouche et al.,] and
investigation of functional oxide materials [Gunnlaugsson et al.]
8.4 Publications since 2009
Below is a list of reviewed publications since 2009. More details can be found on
1. H. P. Gunnlaugsson, K. Johnston, T. E. Mølholt, G. Weyer, R. Mantovan, H.
Masenda, D. Naidoo, S. Ólafsson, K. Bharuth-Ram, H. P. Gíslason, G. Langouche,
M. B. Madsen and the ISOLDE Collaboration, Lattice locations and properties of Fe
in Co/Fe co-implanted ZnO, Appl. Phys. Lett. (2012) Submitted
2. T. E Mølholt, H. P. Gunnlaugsson, K Johnston, R. Mantovan, H. Masenda, D.
Naidoo, S. Ólafsson, K. Bharuth-Ram, H. P. Gislason, G. Langouche, R. Sielemann,
G. Weyer and the ISOLDE Collaboration, Spin-lattice relaxations of paramagnetic
Fe 3+ in ZnO, Physica Scripta (2012) Accepted.
3. H. Masenda, K. Bharuth-Ram, D. Naidoo, H. P. Gunnlaugsson, T. E. Mølholt, H. P.
Gíslason, K. Johnston, R. Mantovan, R. Sielemann, G. Langouche, S. Ólafsson, G.
Weyer, the ISOLDE Collaboration, Mössbauer study of 119 Sn in 119 In ∗ implanted 3C-
SiC, Hyp. Int., (2011) DOI 10.1007/s10751-011-0438-x.
4. K. Bharuth-Ram, W.B. Dlamini, H. Masenda, D. Naidoo, H.P. Gunnlaugsson, G.
Weyer, R. Mantovan, T.E. Mølholt, R. Sielemann, S. Ólafsson, G. Langouche, K.
Johnston, the ISOLDE Collaboration, 57 Fe Mössbauer studies on 57 Mn* implanted
InP and InAs, Nucl. Instr. Meth. B (2011) In press.
5. T. E. Mølholt, R. Mantovan, H.P. Gunnlaugsson, D. Naidoo, S. Ólafsson, K. Bharuth-
Ram, M. Fanciulli, K. Johnston, Y. Kobayashi, G. Langouche, H. Masenda, R.
Sielemann, G. Weyer and H.P. Gíslason, Observation of spin-lattice relaxations of
dilute Fe 3+ in MgO by Mössbauer spectroscopy, Hyp. Int. 197 (2010) 89-94
6. H. P. Gunnlaugsson, R. Sielemann, T.E. Mølholt, W.B. Dlamini, K. Johnston, R.
Mantovan, H. Masenda, D. Naidoo, W. N. Sibanda, K. Bharuth-Ram, M. Fanciulli,
H.P. Gíslason, G. Langouche, S. Ólafsson, G. Weyer and the ISOLDE Collaboration,
Magnetism in iron implanted oxides: a status report, Hyp. Int. 197 (2010) 43-52
7. H. Masenda, D. Naidoo, K. Bharuth-Ram, H.P. Gunnlaugsson, G. Weyer, W.B.
Dlamini, R. Mantovan, R. Sielemann, M. Fanciulli, T.E. Mølholt, S. Ólafsson, G.
Langouche, K. Johnston and the ISOLDE Collaboration, Mössbauer study of 57 Fe in
GaAs and GaP following 57 Mn + implantation, Hyp. Int. 198 (2010) 15-22
8. H. P. Gunnlaugsson, R. Mantovan, T.E. Mølholt, D. Naidoo, K. Johnston, H.
Masenda, K. Bharuth-Ram, G. Langouche, S. Ólafsson, R. Sielemann, G. Weyer, Y.
Kobayashi and the ISOLDE Collaboration, Mössbauer spectroscopy of 57 Fe in α-
Al2O3 following implantation of 57 Mn * , Hyp. Int. 198 (2010) 5-14
9. H. P. Gunnlaugsson, T. E. Mølholt, R. Mantovan, H. Masenda, D. Naidoo, W. B.
Dlamini, R. Sielemann, K. Bharuth-Ram, G. Weyer, K. Johnston, G. Langouche S.
Ólafsson, H. P. Gíslason, Y. Kobayashi, Y. Yoshida, M. Fanciulli and the ISOLDE
Collaboration, Paramagnetism in Mn/Fe implanted ZnO, Appl. Phys. Lett. 97 (2010)
10. T. E. Mølholt, R. Mantovan, H. P. Gunnlaugsson, K. Bharuth-Ram, M. Fanciulli, H.
P. Gíslason, K. Johnston, Y. Kobayashi, G. Langouche, H. Masenda, D. Naidoo, S.
Ólafsson, R. Sielemann, G. Weyer, Temperature and dose dependence of defect
complex formation with ion-implanted Mn/Fe in ZnO, Physica B 404 (2009) 4820-
4822, doi: 10.1016/j.physb.2009.08.187.
11. K. Bharuth-Ram, H. P. Gunnlaugsson, G. Weyer, R. Mantovan, D. Naidoo, R.
Sielemann, M. Fanciulli, G. Langouche, S. Olafsson, Th. Aigne, ISOLDE
Collaboration, Mössbauer study of Fe in GaAs following 57 Mn + implantation, Hyp.
Int. 119 (2009) 115–120, doi: 10.1007/s10751-009-9961-4
12. H. P. Gunnlaugsson, G. Weyer, R. Mantovan, D. Naidoo, R. Sielemann, K. Bharuth-
Ram, M. Fanciulli, K. Johnston, S. Olafsson, G. Langouche, Isothermal defect
annealing in semiconductors investigated by time-delayed Mössbauer spectroscopy:
application to ZnO, Hyperfine Interact. 188 (2009) 85–89, doi: 10.1007/s10751-008-
13. D. Naidoo, H. P. Gunnlaugsson, K. Bharuth-Ram, V. V. Naicker, G. Weyer, R.
Sielemann, R. Mantovan, M. Fanciulli, the ISOLDE Collaboration, 57 Fe Mössbauer
Investigations in P-Type Silicon Germanium Single Crystals. Hyp. Int. 188 (2009)
11-17, doi: 10.1007/s10751-008-9880-9
8.5 Research degrees completed/to be submitted (since 2008):
PhD: R Mantovan, University of Milan, Italy, 2008
D. Naidoo, University of KwaZulu-Natal, South Africa, 2008
T E Molholt, University of Iceland, (to submit in 2012)
MSc: H. Masenda, University of the Witwatersrand, South Africa, 2010
Ms W B Dlamini, University of KwaZulu-Natal, South Africa, 2011.
9 Appendix 3: Description of the proposed experiment
The experimental setup comprises: Mössbauer setup, stored outside the hall when not in
Part of the Choose an item. Availability Design and manufacturing
Mössbauer setup Existing To be used without any modification
SSP-GLM chamber Existing To be used without any modification
9.1 Hazards generated by the experiment
To be modified
New Standard equipment supplied by a manufacturer
CERN/collaboration responsible for the design and/or
Mössbauer setup SSP-GLM chamber [Part 3 of the
Thermodynamic and fluidic
Pressure Low pressure only Low pressure only
Vacuum Yes Yes
Temperature < 100 o C (outside setup) Room temperature
Heat transfer No No
Thermal properties of
Cryogenic fluid N 2, 1[Bar], 3 l/h N/A
Electrical and electromagnetic
Dose rate on contact
and in 10 cm distance
Activity ~50 mCi (inside the setup)
UV light No No
Toxic No No
Harmful No No
mutagens and substances
toxic to reproduction)
Corrosive No No
Irritant No No
Flammable No No
Oxidizing No No
Explosiveness No No
Asphyxiant No No
Dangerous for the
Physical impact or
mechanical energy (moving
(Sharp, rough, slippery)
Vibration No No
Vehicles and Means of
Frequency No No
Intensity No No
Confined spaces No No
High workplaces No No
Access to high workplaces No No
Just outside GLM No
Manual handling ? ?
Poor ergonomics ? ?
0.5 Hazard identification
4-10 µCi (0.15-0.4 MBq)
3.2 Average electrical power requirements (excluding fixed ISOLDE-installation mentioned
above): ~200 W during on-line experiments